- Nano Express
- Open Access
Three-dimensional MoS2/Graphene Aerogel as Binder-free Electrode for Li-ion Battery
Nanoscale Research Letters volume 14, Article number: 85 (2019)
Hybrid MoS2/reduced graphene aerogels with rich micro-pore are fabricated through a hydrothermal method, followed by freeze-drying and annealing treatment. The porous structure could act as an electrode directly, free of binder and conductive agent, which promotes an improved electron transfer, and provides a 3D network for an enhanced ion transport, thus leading to an increased capacity and stable long cycle stability performance. Notably, the specific capacity of MoS2/reduced graphene aerogel is 1041 mA h g−1 at 100 mA g−1. Moreover, reversible capacities of 667 mA h g−1 with 58.6% capacity retention are kept after 100 cycles. The outstanding performance is beneficial from the synergistic effect of the MoS2 nanostructure and graphene conductive network, as well as the binder-free design. These results provide a route to integrate transition-metal-dichalcogenides with graphene to fabricate composites with rich micro-pores and a three-dimensional network for energy storage devices.
Nowadays, the rapid development of electric vehicles and flexible electronics opens up an opportunity for the development of energy storage devices in the industrial and research communities [1, 2]. Among the various energy storage devices, lithium ion batteries (LIBs) are paid more attention due to their outstanding energy storage capability as well as long cycle life [3,4,5].
Recently, many researches have focused on high-performance anode materials for LIBs. 2D transition metal dichalcogenides (TMDs), with outstanding electrochemical performance, have won much attention and showed great potential as anode materials for LIBs [6, 7]. Comparing with conventional metal oxides, the metal sulfides with higher conductivity and larger interlayer spacing promote an improved electron transfer and enhanced ion transport . Among the metal sulfides, molybdenum disulfide (MoS2) shows great advantages as the anode of LIBs due to its unique layered structure and high capacity (ca. 670 mAh g−1). However, its structure is prone to deteriorate during the charge/discharge process due to volume change, leading to a poor cycling stability. Numerous attempts have been conducted to enhance kinetic behaviors of MoS2 as LIBs anode. One method is to synthesis nano-size structure, in order to shorten the diffusion distance of lithium ions [9, 10]. Another method is to incorporate carbon materials to improve the composite conductivity and repress the volume expansion during charge/discharge process [11,12,13]. Different carbon materials [14,15,16,17,18,19,20], including carbon nanotubes  and graphene [19, 20], are used to integrate with MoS2 and it proves to be in effect. Especially, graphene has drawn much attention benefiting from its outstanding conductivity and high surface area. Recently, graphene has been widely researched in many areas, such as conductive switching , photoluminescence , chemical cleaning , and gas sensing  as well as energy storage fields . For instance, Teng et al. prepared MoS2 nanosheets on graphene sheets, and a capacity of 1077 mAh g−1 at 100 mA g−1 after 150 cycles was obtained . Liu et al. fabricated a composite of MoS2 and graphene , and the reversible capacity of 1300–1400 mAh g−1 was obtained. How to incorporate graphene with MoS2 to obtain the high-capacity and stable anode material is still an ongoing task .
Herein, a facile and low-cost approach is used to prepare a hierarchical nanostructure of MoS2/reduced graphene (MoS2/RGO) aerogel. With a solvothermal and freezing-drying process, the MoS2/RGO aerogel is fabricated and directly acts as the binder-free anode. Such a structure endows the MoS2/graphene aerogel with several advantages as an anode material. First, the graphene acts as a matrix to support the MoS2 nanostructures, which is beneficial to preventing graphene sheets from restacking. Second, the hierarchical nanostructure provides a good adhesion between graphene and MoS2, which ensure a stable structure and thus guarantee a long cycling stability. Third, the graphene with high conductivity promotes an improved electron transfer and acts as a basis to alleviate volume expansion of MoS2 in the charge/discharge process. Fourth, such a binder-free design shortens the ion diffusion distance, leading to an enhanced ion transport. The reversible capacity of the as-prepared binder-free MoS2/RGO aerogel is up to 667 mA h g−1 at 100 mA g−1 after 100 cycles. This method provides a route to fabricate the high-performance lithium-ion anode material.
Materials and Methods
Synthesis of MoS2/RGO Aerogels
All reagents were of analytical grade. A modified Hummers’ method was used to prepare graphene oxide (GO) for further use . The MoS2/RGO aerogels were prepared with a one-step hydrothermal method. In detail, 60 mg of (NH4)2MoS4 were dissolved in 10 mL of N, N-dimethylformamide (DMF) solvent. Five milliliters of GO aqueous (5 mg mL−1) were added, and a homogeneous solution was obtained under sonication for several hours. The solution was put to a Teflon-lined autoclave and sealed. Finally, it was heated in the oven at 200°C for 12 h. MoS2/RGO hydrogels were obtained through washing with ethanol and D.I. water. Through freeze-drying and annealing in 700°C for 2 h, the final MoS2/RGO aerogels were obtained. As a comparison, the MoS2 powder was prepared with the same steps except adding GO.
A thin piece of MoS2/RGO film which was cut from the MoS2/RGO aerogels was used to carry out further characterization. Field mission scanning electron microscopy (FESEM, JEOL JSM-6700F) and field-emission transmission electron microscopy (FETEM, FEI, Tecnai G2 F30) were used to characterize the obtained samples. XRD analysis (PANalytical PW3040/60) with Cu Kα radiation (λ = 1.5406 Å) from 10° to 80° was used to confirm the substance of the MoS2/RGO film and MoS2 powder.
The MoS2/RGO film was directly used as a binder-free anode, without any binder and conductive agent. It was assembled into a coin-type half-cell in a glove box, with a lithium foil acting as counter electrode and Celgard 2400 polymer as separator. The electrolyte consisted of 1 M LiPF6 in ethylene carbonate (EC) and diethyl carbonate (DEC). After assembly, the cell was aged 24 h in the glove box for further measurements. The galvanostatic charge/discharge (GCD) measurements were carried out with a battery measurement system (Land, China), and cyclic voltammetry (CV) testings were conducted with Autolab workstation (PGSTAT-302N). The testing was conducted in the potential range of 0.01–3.0 V (vs Li1/Li). Electrochemical impedance spectra (EIS) experiments were carried out with 10 mV amplitude in the frequency from 100 kHz to 0.01 Hz.
Results and Discussion
The MoS2/RGO aerogels were fabricated with a hydrothermal method, freeze-drying and heat treatment. Figure 1 displayed the preparation process of the MoS2/RGO electrode. Detailed methods were described on the Materials and methods. As shown in Additional file 1: Figure S1 and Additional file 2: Figure S2, the obtained MoS2/RGO aerogel could keep integrate structure. The excellent mechanical behavior was beneficial from the rich porosity of the whole structure and the interconnection of graphene layers, showing great potential as a binder-free electrode.
Figure 2 presented the morphology of MoS2/rGO aerogel. A porous structure with wrinkled graphene layers interconnected with each other was observed (Fig. 2a), where MoS2 nanostructures covered the whole graphene layers. The microstructure of MoS2/RGO aerogels was further confirmed with TEM (Additional file 3: Figure S3). As displayed in Fig. 2c and d, the MoS2 nanostructures were distributed on the graphene even after long-time ultrasonication, illustrating the strong interaction of MoS2 on graphene. The high-resolution TEM image was displayed in Fig. 2f. The graphene layers were covered with MoS2 nanostructures, where lattice spacings of 0.61 and 0.27 nm were observed, which were responsible for (002) and (100) planes of MoS2 . The SAED pattern (inset of Fig. 2f) presented several diffraction rings, which was well corresponding to MoS2 planes . These results illustrated that MoS2 nanostructures on graphene layer exhibited a good crystallinity. The elemental distribution of the aerogel was detected (Fig. 2g–j) where Mo, S, and C elements were almost overlapped with the whole structure, suggesting the successful fabrication of the composite.
X-ray diffraction (XRD) experiments were also carried out. As shown in Fig. 3a, the XRD patterns of the MoS2 powder could be responsible for hexagonal 2H–MoS2 (JCPDS 37-1492). The strong reflection peak at 2θ = 14.2o belonged to the (002) plane, with a d-spacing of 0.62 nm. MoS2/RGO composite showed the similar crystalline structure of pure MoS2, indicating a layered structure. Comparing with the MoS2 samples, an obvious peak in 26.3° was observed in the MoS2/RGO samples, which could be the (002) diffraction peak of graphene, revealing the graphene substance in the composites . It was worth pointing out that the obvious peak at 14.4°, 32.7° and 58.3° were ascribed to the (002), (100) and (110) diffraction peak of MoS2, which was consistent with the previous SAED pattern results. Notably, the MoS2 (002) reflection peak, which indicated a stacked nature of layered MoS2, was weakened for the MoS2/RGO composite, suggesting the formation of a few-layer MoS2 structure [26, 32]. The peaks of graphene were more obvious than the MoS2, further confirming that the MoS2 was wrapped by graphene layer in the MoS2/RGO aerogels [26, 32].
To further confirm the nature of MoS2 nanostructure and graphene layer, Raman spectroscopy measurements were also carried out [33,34,35]. As shown in Fig. 3b, the MoS2/RGO aerogel showed the E2g and A1g peaks of MoS2 at the frequencies of 380.2 and 403.6 cm−1 [18, 36]. Notably, it had been reported that the single-layer MoS2 nanostructure with different fabrication method would display an A1g peak at 402–404 cm−1 [37,38,39], further identifying the few layer of MoS2 crystals in the MoS2/RGO aerogel. Besides, the peaks at 1354.3 cm−1 and 1591.6 cm−1 were observed in Fig. 3b, which were characteristic peaks of the D- and G-bands of graphene [40,41,42]. The intensity ratio ID/IG was usually associated with the graphene defects . The value was calculated to be 1.08, indicating the reduced graphene with some defects .
To demonstrate the performance of MoS2/RGO electrode, CV measurements at a scan rate of 0.5 mV s−1 were carried out. Figure 4a showed the first three CV curves of MoS2/RGO composite. A broad shoulder peak was observed at 0.95 V when there were reduction peaks at 0.65 V in the first cathodic sweep of the MoS2/RGO electrode. The peak at 0.95 V was related with Li+ intercalation into MoS2 interlayer space to form LixMoS2, with a phase transformation process to become 1T(octahedral) structure of LixMoS2 from 2H (trigonal prismatic) [43, 44]. The other peak at 0.65 V was accompanied with the process to form Li2S and metallic Mo from LixMoS2 [45,46,47]. In the following discharge scans, there were reduction peaks located at 1.80 V and 1.05 V, indicating a different reaction process. One pronounced peak at 2.34 V was observed for the MoS2/RGO electrode in the reverse anodic scans, indicating the formation of sulfur . It could be inferred that sulfur, Mo, and few MoS2 were formed after the first cycle and they were kept the same in subsequent cycles [36, 48,49,50]. In addition, the discharge curves were identical except for the first one, indicating the electrochemical stability for the MoS2/RGO composite. The first three GCD curves of the MoS2/RGO and MoS2 electrodes were shown in Fig. 4b and c. In the first discharge cycle of the MoS2 electrode, two potential plateaus were observed at 1.05 V and 0.65 V (Fig. 4b). The 1.05 V plateau was accompanied with the process of forming LixMoS2, and the plateau at 0.65 V was related with the reaction of forming Mo particles from MoS2. A slope potential curve was observed below 0.52 V in the first discharge cycles, meaning the appearance of gel-like polymeric layer due to the degradation of electrolyte [51,52,53]. The MoS2 electrode showed plateaus at 2.0, 1.20 and 0.45 V in the following discharge curves. In the charge process, an obvious plateau at 2.35 V was observed for the MoS2 electrode. For the MoS2/RGO electrode (Fig. 4c), there was no obvious potential plateau during the first discharge cycle, except for a week plateau at 1.1–0.6 V, which was mainly ascribed to the overlapping lithium process in MoS2 and RGO . MoS2/RGO electrode displayed a plateau at 1.95 V in the following discharge cycles, in agreement with the CV results. During the charge cycles, the MoS2/RGO electrode showed a plateau at 2.2 V. Figure 4c showed the discharge and charge capacity of MoS2/RGO and MoS2 electrode. MoS2/RGO electrode delivered 2215 mAh g−1 discharge capacity in the first discharge cycle, with a reversible charge capacity of 1202 mAh g−1. The corresponding values for the MoS2 were 671.1 mAh g−1 and 680.5 mAh g−1, respectively. The irreversible processes in the first cycle, such as decomposition of electrolyte and the formation of SEI film, lead to irreversibility [55, 56].
The rate performances of MoS2/RGO electrode and MoS2 electrodes were shown in Fig. 4d. Comparing with single MoS2 electrodes, MoS2/RGO electrodes delivered higher capacities. A capacity of 1041 mAh g−1 at 100 mA g−1 was kept after 50 discharge/charge cycles for the MoS2/RGO electrode, indicating a good electrochemical reversibility as well as a long cycle stability. By comparison, the MoS2 electrode only kept 512 mAh g−1 capacity at 100 mA g−1 after 50 cycles. Moreover, the specific capacity of the MoS2 electrode decreased a lot when the current decreased from 2000 mA g−1 to100 mA g−1. The cycling results conducted at 100 mA g−1 were shown in Fig. 4e. The MoS2 electrode showed a poor cycling performance. There was nearly no decrease in its initial 20 cycles. However, the reversible (charge) capacity decreased from 892 mAh g−1 to 110 mAh g−1 after 100 cycles, with only 12.3% capacity retention. On the contrary, the MoS2/RGO electrodes displayed an improved cyclic stability. A reversible capacity of 667 mAh g−1, with a 58.6% capacity retention was obtained after 100 cycles. The rate performances and cycling stability of pure RGO electrode were also displayed in Additional file 4: Figure S4. The RGO electrode delivered a reversible charge capacity of 297.8 mAh g−1 at 100 mA g−1. When the current density reversed from 2000 mA g−1 to100 mA g−1, the specific capacity of 202.2 mAh g−1 was kept for the RGO electrode. Table 1 showed a comparison of the capacity performance about the binder-free MoS2/RGO and other materials based on MoS2/rGO listed in the literature [57,58,59,60,61,62,63]. It could be seen that the binder-free MoS2/RGO electrode showed high capacity compared with other porous MoS2/RGO composites ever reported. These results illustrated the successful introduction of RGO, and the important role it played in the delithium-lithium process . Firstly, the graphene layer with highly porous architecture provided rich active sites for the MoS2 nanostructure, which was beneficial to preventing aggregation of MoS2. Secondly, the graphene with good conductivity reduced transfer resistance and promoted electron transmission and ion transport, leading to an improved rate capability. Thirdly, the RGO aerogel with multi-scale porous structure acted as an elastic buffer layer, which effectively restrained the volume expansion during the delithium-lithium process, and thus lead a better cycling stability.
Electrochemical impedance spectra (EIS) measurements were also conducted for the samples. Figure 5a showed the Nyquist plots of MoS2/RGO and MoS2 electrodes after 100 discharge-charge cycles at 100 mA g−1. The first semicircle represented lithium ion migration resistance through the SEI films (R1), while the second semicircle stood for the resistance of charge transport (Rct). R2 was related with the resistance of electrolyte . ZView software was used to fit the curves of MoS2/RGO and MoS2 electrodes. The fitted values were listed in the Fig. 5b. From the table, the Rct of the MoS2/RGO electrode (10.74Ω) was smaller than MoS2 (44.07 Ω), indicating that rGO could bring an improved charge transfer process during discharge-charge actions and thus show a good rate capability.
To investigate the impact of repeated charge/discharge processes on the as-prepared samples, FESEM were conducted on the samples after 100 cycles at 100 mA g−1 (Additional file 1: Figure S1). MoS2/ RGO electrode kept a well structure without any cracks. The cross-sectional FESEM pictures in Additional file 1: Figure S1c and d showed the high-compressible graphene layer where nanoparticles were distributed. On the contrary, severe cracks were observed on the pristine MoS2 electrode in Additional file 1: Figure S1e and f. It was mainly because the volume expansion of active material during cycling, thus leading to particles aggregation. The above results illustrated the important role of graphene layer in inhibiting the volume expansion in the cycling process (Additional file 5: Figure S5).
In summary, hybrid MoS2/RGO aerogels with rich micropores have been fabricated. The prepared aerogels are used as electrodes without any binder and conducting agent. Such a nanostructure design with abundant micro-pores is not only beneficial to providing 3D network for enhanced electron transfer, but also can shorten the transport distance, thus leading to an improved electrochemical rate and stable performance as the anode electrodes for LIBs. MoS2/RGO aerogel delivers specific capacities of 1041 mA h g−1 at 100 mA g−1, which is ascribed to the synergistic effect of MoS2 nanostructure and conductive graphene, as well as the binder-free design with abundant micro-pores. The study offers useful insights for realizing high-performance anode electrodes for LIBs with high capacity and long cycle stability.
Electrochemical impedance spectroscopy
Lithium ion batteries
- MoS2 :
MoS2/ reduced graphene
Lithium ion migration resistance through the SEI films
The resistance of electrolyte
The resistance of charge transport
Selected area electron diffraction
2D transition metal dichalcogenides
Armand M, Tarascon J-M (2008) Building better batteries. Nature 451:652–657
Scrosati B, Hassoun J, Sun Y-K (2011) Lithium-ion batteries. A look into the future. Energy Environ Sci 4:3287–3295
Kim SW, Seo DH, Ma X, Ceder G, Kang K (2012) Electrode materials for rechargeable sodium-ion batteries: potential alternatives to current lithium-ion batteries. Adv Energy Mater 2:710–721
Yabuuchi N, Kubota K, Dahbi M, Komaba S (2014) Research development on sodium-ion batteries. Chem Rev 114:11636–11682
David L, Bhandavat R, Barrera U, Singh G (2016) Silicon oxycarbide glass-graphene composite paper electrode for long-cycle lithium-ion batteries. Nat Commun 7:10998 https://doi.org/10.1038/ncomms10998
Tan C, Zhang H (2015) Two-dimensional transition metal dichalcogenide nanosheet-based composites. Chem Soc Rev 44:2713–2731
Zhu C, Mu X, van Aken PA, Yu Y, Maier J (2014) Single-layered ultrasmall nanoplates of MoS2 embedded in carbon nanofibers with excellent electrochemical performance for lithium and sodium storage. Angew Chem Int Ed 53:2152–2156
Zhu C, Mu X, van Aken PA, Maier J, Yu Y (2015) Fast Li storage in MoS2-graphene-carbon nanotube nanocomposites: advantageous functional integration of 0D, 1D, and 2D nanostructures. Adv Energy Mater 5(4):1401170
Liu C, Li F, Ma LP, Cheng HM (2010) Advanced materials for energy storage. Adv Mater 22(8):E28-E62.
Wu Z-S, Zhou G, Yin L-C, Ren W, Li F, Cheng H-M (2012) Graphene/metal oxide composite electrode materials for energy storage. Nano Energy 1:107–131
Reddy M, Subba Rao G, Chowdari B (2013) Metal oxides and oxysalts as anode materials for Li ion batteries. Chem Rev 113:5364–5457
Ji L, Lin Z, Alcoutlabi M, Zhang X (2011) Recent developments in nanostructured anode materials for rechargeable lithium-ion batteries. Energy Environ Sci 4:2682–2699
Guo YG, Hu JS, Wan LJ (2008) Nanostructured materials for electrochemical energy conversion and storage devices. Adv Mater 20:2878–2887
Chang K, Chen W, Ma L, Li H, Li H, Huang F, Xu Z, Zhang Q, Lee J-Y (2011) Graphene-like MoS 2/amorphous carbon composites with high capacity and excellent stability as anode materials for lithium ion batteries. J Mater Chem 21:6251–6257
Wang C, Wan W, Huang Y, Chen J, Zhou HH, Zhang XX (2014) Hierarchical MoS 2 nanosheet/active carbon fiber cloth as a binder-free and free-standing anode for lithium-ion batteries. Nanoscale 6:5351–5358
Wan Z, Shao J, Yun J, Zheng H, Gao T, Shen M, Qu Q, Zheng H (2014) Core–shell structure of hierarchical quasi-hollow MoS2 microspheres encapsulated porous carbon as stable anode for Li-ion batteries. Small 10:4975–4981
Zhang L, Lou XWD (2014) Hierarchical MoS2 shells supported on carbon spheres for highly reversible lithium storage. Chem Eur J 20:5219–5223
Shi Y, Wang Y, Wong JI, Tan AYS, Hsu C-L, Li L-J, Lu Y-C, Yang HY (2013) Self-assembly of hierarchical MoSx/CNT nanocomposites (2<x<3): towards high performance anode materials for lithium ion batteries. Sci Rep 3:2169 https://doi.org/10.1038/srep02169
Wang J, Liu J, Chao D, Yan J, Lin J, Shen ZX (2014) Self-assembly of honeycomb-like MoS2 nanoarchitectures anchored into graphene foam for enhanced lithium-ion storage. Adv Mater 26:7162–7169
Wang Y, Kong D, Shi W, Liu B, Sim GJ, Ge Q, Yang HY (2016) Ice templated free-standing hierarchically WS2/CNT-rGO aerogel for high-performance rechargeable lithium and sodium ion batteries. Adv Energy Mater 6(21):1601057
Wei J, Zang Z, Zhang Y, Wang M, Du J, Tang X (2017) Enhanced performance of light-controlled conductive switching in hybrid cuprous oxide/reduced graphene oxide (Cu 2 O/rGO) nanocomposites. Opt Lett 42:911–914
Zang Z, Zeng X, Wang M, Hu W, Liu C, Tang X (2017) Tunable photoluminescence of water-soluble AgInZnS–graphene oxide (GO) nanocomposites and their application in-vivo bioimaging. Sensors Actuators B Chem 252:1179–1186
Huang H, Zhang J, Jiang L, Zang Z (2017) Preparation of cubic Cu2O nanoparticles wrapped by reduced graphene oxide for the efficient removal of rhodamine B. J Alloys Compd 718:112–115
Liu J, Li S, Zhang B, Xiao Y, Gao Y, Yang Q, Wang Y, Lu G (2017) Ultrasensitive and low detection limit of nitrogen dioxide gas sensor based on flower-like ZnO hierarchical nanostructure modified by reduced graphene oxide. Sensors Actuators B Chem 249:715–724
Ramadoss A, Yoon K-Y, Kwak M-J, Kim S-I, Ryu S-T, Jang J-H (2017) Fully flexible, lightweight, high performance all-solid-state supercapacitor based on 3-dimensional-graphene/graphite-paper. J Power Sources 337:159–165
Teng Y, Zhao H, Zhang Z, Li Z, Xia Q, Zhang Y, Zhao L, Du X, Du Z, Lv P (2016) MoS2 Nanosheets vertically grown on graphene sheets for lithium-ion battery anodes. ACS Nano 10:8526–8535
Liu Y, Zhao Y, Jiao L, Chen J (2014) A graphene-like MoS 2/graphene nanocomposite as a highperformance anode for lithium ion batteries. J Mater Chem A 2:13109–13115
Hummers WS Jr, Offeman RE (1958) Preparation of graphitic oxide. J Am Chem Soc 80:1339–1339
Chang K, Chen W (2011) In situ synthesis of MoS 2/graphene nanosheet composites with extraordinarily high electrochemical performance for lithium ion batteries. Chem Commun 47:4252–4254
Hou Y, Wen Z, Cui S, Guo X, Chen J (2013) Constructing 2D porous graphitic C3N4 nanosheets/nitrogen-doped graphene/layered MoS2 ternary nanojunction with enhanced photoelectrochemical activity. Adv Mater 25:6291–6297
Zhao L, Hong C, Lin L, Wu H, Su Y, Zhang X, Liu A (2017) Controllable nanoscale engineering of vertically aligned MoS 2 ultrathin nanosheets by nitrogen doping of 3D graphene hydrogel for improved electrocatalytic hydrogen evolution. Carbon 116:223–231
Hwang H, Kim H, Cho J (2011) MoS2 nanoplates consisting of disordered graphene-like layers for high rate lithium battery anode materials. Nano Lett 11:4826–4830
Kudin KN, Ozbas B, Schniepp HC, Prud’Homme RK, Aksay IA, Car R (2008) Raman spectra of graphite oxide and functionalized graphene sheets. Nano Lett 8:36–41
Caballero Á, Morales J (2012) Can the performance of graphene nanosheets for lithium storage in Li-ion batteries be predicted? Nanoscale 4:2083–2092
Pimenta M, Dresselhaus G, Dresselhaus MS, Cancado L, Jorio A, Saito R (2007) Studying disorder in graphite-based systems by Raman spectroscopy. Phys Chem Chem Phys 9:1276–1290
Frey GL, Tenne R, Matthews MJ, Dresselhaus M, Dresselhaus G (1999) Raman and resonance Raman investigation of MoS 2 nanoparticles. Phys Rev B 60:2883
Ghatak S, Pal AN, Ghosh A (2011) Nature of electronic states in atomically thin MoS2 field-effect transistors. ACS Nano 5:7707–7712
Lee C, Yan H, Brus LE, Heinz TF, Hone J, Ryu S (2010) Anomalous lattice vibrations of single-and few-layer MoS2. ACS Nano 4:2695–2700
Lee HS, Min S-W, Chang Y-G, Park MK, Nam T, Kim H, Kim JH, Ryu S, Im S (2012) MoS2 nanosheet phototransistors with thickness-modulated optical energy gap. Nano Lett 12:3695–3700
Xiong X, Wang G, Lin Y, Wang Y, Ou X, Zheng F, Yang C, Wang J-H, Liu M (2016) Enhancing sodium ion battery performance by strongly binding nanostructured Sb2S3 on sulfur-doped graphene sheets. ACS Nano 10:10953–10959
Xiang H, Li Z, Xie K, Jiang J, Chen J, Lian P, Wu J, Yu Y, Wang H (2012) Graphene sheets as anode materials for Li-ion batteries: preparation, structure, electrochemical properties and mechanism for lithium storage. RSC Adv 2:6792–6799
Wang Z, Chen T, Chen W, Chang K, Ma L, Huang G, Chen D, Lee JY (2013) CTAB-assisted synthesis of single-layer MoS 2–graphene composites as anode materials of Li-ion batteries. J Mater Chem A 1:2202–2210
Li X-L, Li Y-D (2004) MoS2 nanostructures: synthesis and electrochemical Mg2+ intercalation. J Phys Chem B 108:13893–13900
Liu Y, He X, Hanlon D, Harvey A, Khan U, Li Y, Coleman JN (2016) Electrical, mechanical, and capacity percolation leads to high-performance MoS2/nanotube composite lithium ion battery electrodes. ACS Nano 10:5980–5990
Fang Y, Lv Y, Gong F, Elzatahry AA, Zheng G, Zhao D (2016) Synthesis of 2D-mesoporous-carbon/MoS2 heterostructures with well-defined interfaces for high-performance lithium-ion batteries. Adv Mater 28:9385–9390
Wang Y, Yu L, Lou XWD (2016) Inside back cover: synthesis of highly uniform molybdenum–glycerate spheres and their conversion into hierarchical MoS2 hollow nanospheres for lithium-ion batteries (Angew. Chem. Int. Ed. 26/2016). Angew Chem Int Ed 55:7549–7549
Jiang L, Lin B, Li X, Song X, Xia H, Li L, Zeng H (2016) Monolayer MoS2–graphene hybrid aerogels with controllable porosity for lithium-ion batteries with high reversible capacity. ACS Appl Mater Interfaces 8:2680–2687
Deng Z, Jiang H, Hu Y, Liu Y, Zhang L, Liu H, Li C (2017) 3D ordered macroporous MoS2@ C nanostructure for flexible Li-ion batteries. Adv Mater 29(10):1603020.
Chao Y, Jalili R, Ge Y, Wang C, Zheng T, Shu K, Wallace GG (2017) Self-assembly of flexible free-standing 3D porous MoS2-reduced graphene oxide structure for high-performance Lithium-ion batteries. Adv Funct Mater 27(22):1700234.
Wang R, Wang S, Peng X, Zhang Y, Jin D, Chu PK, Zhang L (2017) Elucidating the intercalation pseudocapacitance mechanism of MoS2–carbon monolayer interoverlapped superstructure: toward high-performance sodium-ion-based hybrid supercapacitor. ACS Appl Mater Interfaces 9:32745–32755
Chang K, Chen W (2011) L-cysteine-assisted synthesis of layered MoS2/graphene composites with excellent electrochemical performances for lithium ion batteries. ACS Nano 5:4720–4728
Zuo X, Chang K, Zhao J, Xie Z, Tang H, Li B, Chang Z (2016) Bubble-template-assisted synthesis of hollow fullerene-like MoS 2 nanocages as a lithium ion battery anode material. J Mater Chem A 4:51–58
Zhou J, Qin J, Zhao N, Shi C, Liu E-Z, He F, Li J, He C (2016) Salt-template-assisted synthesis of robust 3D honeycomb-like structured MoS 2 and its application as a lithium-ion battery anode. J Mater Chem A 4:8734–8741
Cao X, Shi Y, Shi W, Rui X, Yan Q, Kong J, Zhang H (2013) Preparation of MoS2-coated three-dimensional graphene networks for high-performance anode material in Lithium-ion batteries. Small 9:3433–3438
Huang G, Chen T, Chen W, Wang Z, Chang K, Ma L, Huang F, Chen D, Lee JY (2013) Graphene-like MoS2/graphene composites: cationic surfactant-assisted hydrothermal synthesis and electrochemical reversible storage of lithium. Small 9:3693–3703
Zhou J, Qin J, Zhang X, Shi C, Liu E, Li J, Zhao N, He C (2015) 2D space-confined synthesis of few-layer MoS2 anchored on carbon nanosheet for lithium-ion battery anode. ACS Nano 9:3837–3848
Li H, Yu K, Fu H, Guo B, Lei X, Zhu Z (2015) MoS2/graphene hybrid nanoflowers with enhanced electrochemical performances as anode for lithium-ion batteries. J Phys Chem C 119:7959–7968
Liu H, Chen X, Deng L, Su X, Guo K, Zhu Z (2016) Preparation of ultrathin 2D MoS 2/graphene heterostructure assembled foam-like structure with enhanced electrochemical performance for lithium-ion batteries. Electrochim Acta 206:184–191
Youn DH, Jo C, Kim JY, Lee J, Lee JS (2015) Ultrafast synthesis of MoS2 or WS2-reduced graphene oxide composites via hybrid microwave annealing for anode materials of lithium ion batteries. J Power Sources 295:228–234
Choi M, Koppala SK, Yoon D, Hwang J, Kim SM, Kim J (2016) A route to synthesis molybdenum disulfide-reduced graphene oxide (MoS2-RGO) composites using supercritical methanol and their enhanced electrochemical performance for Li-ion batteries. J Power Sources 309:202–211
Jing Y, Ortiz-Quiles EO, Cabrera CR, Chen Z, Zhou Z (2014) Layer-by-layer hybrids of MoS 2 and reduced graphene oxide for lithium ion batteries. Electrochim Acta 147:392–400
Srivastava S, Kartick B, Choudhury S, Stamm M (2016) Thermally fabricated MoS2-graphene hybrids as high performance anode in lithium ion battery. Mater Chem Phys 183:383–391
Zhang X, Zhang Q, Sun Y, Zhang P, Gao X, Zhang W, Guo J (2016) MoS2-graphene hybrid nanosheets constructed 3D architectures with improved electrochemical performance for lithium-ion batteries and hydrogen evolution. Electrochim Acta 189:224–230
We thank the Analytical and Testing Center of Huazhong University of Science and Technology (HUST) for the field emission scanning electron microscopy (FESEM) testing, as well as Flexible Electronics Research Center of HUST.
This work is supported by the National Science Foundation of China (No. 51275195 and No.51775218), the National Basic Research Program of China (No. 2015CB057205), the Program for Changjiang Scholars.
Availability of Data and Materials
All datasets are presented in the main paper or in the additional supporting files.
The authors declare that they have no competing interests and the mentioned received funding in our manuscript does not lead to any conflict of interests regarding the publication of this work.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Figure S1. Mechanical performance of the MoS2/RGO aerogel under the finger compression. (JPG 70 kb)
Figure S2. Mechanical performance of the MoS2/RGO aerogel before compression (a), under compression (b), and after compression (c). (PNG 2203 kb)
Figure S3. (a) TEM picture of the MoS2/RGO sample. (b) TEM-EDS mapping of Mo, S, C elements. (c) EDX spectra of the MoS2/RGO sample. (JPG 304 kb)
Figure S4. (a) Rate performances of RGO aerogel electrodes at different current densities. (b) Cycling performance of RGO electrodes at a constant current density of 100 mA g−1. (JPG 114 kb)
Figure S5. FESEM images of (a, b) MoS2/RGO electrode, (c, d) cross-sectional images of MoS2/RGO and SEM images of (e, f) bare MoS2 electrode after 100 cycles performed with a current density of 100 mA g−1. (JPG 1649 kb)
About this article
Cite this article
Zhong, Y., Shi, T., Huang, Y. et al. Three-dimensional MoS2/Graphene Aerogel as Binder-free Electrode for Li-ion Battery. Nanoscale Res Lett 14, 85 (2019) doi:10.1186/s11671-019-2916-z
- Graphene aerogel
- Li-ion battery